Research Article  Open Access
Qi Hong, Yaoyao Shi, "Multiresponse Parameter Optimization for the Composite Tape Winding Process Based on GRA and RSM", Mathematical Problems in Engineering, vol. 2020, Article ID 2515014, 11 pages, 2020. https://doi.org/10.1155/2020/2515014
Multiresponse Parameter Optimization for the Composite Tape Winding Process Based on GRA and RSM
Abstract
Composite tape winding is an important forming process of composite materials, which can ensure good performance of composite products. Selection and control of key process parameters in the winding process have a great influence on the properties of products, such as void content and residual stress of products. Through experimental analysis, the residual stress and void content of the composite products are not the minimum when the prepreg winding process is carried out by using the empirical process parameters. To solve this multiobjective optimization problem, experiments were conducted using the Box–Behnken design. The multiobjective optimization problem is converted to a singleobjective problem using grey relational analysis (GRA). Principal component analysis (PCA) is used to quantify the relative contributions of residual stress and void content. Regression analysis of grey relational grade (GRG) based on the experimental data was used to develop a secondorder GRG prediction model. The winding process parameters were optimized with response surface methodology (RSM), and the winding experiments were carried out with these parameters. The experimental results show that the best combination of process parameters yields the best GRG results with better void content and residual stress.
1. Introduction
Due to good mechanical, chemical, and physical properties, composite materials are increasingly used. Advanced resin matrix composites have been widely used in the manufacture of solid rocket motor nozzles, parts of ablation and thermal protection materials, launch tubes, and special equipment for the spacecraft. They have many advantages including low density, high strength and stiffness ratios, good corrosion resistance, and ease of integral molding [1–3]. The properties of composite prepreg tape winding products depend on the properties of the materials themselves, molding process parameters, and control accuracy. Therefore, controlling the winding process and the process parameters is the key to ensuring the products have the desired properties. The main parameters in the composite prepreg tape winding process include winding temperature, tension, force, and winding speed [4–8]. An adaptive genetic algorithm with minimum product weight is proposed in [9, 10], and RSM (RSM is a statistical method to solve multivariable problems, multiple quadratic regression equations which are used to fit the functional relationship between factors and response values, and through the analysis of regression equations to find the optimal process parameters) is used to predict the strength reliability of the composite material in highpressure hydrogen storage vessels. One study analyzed the coupling mechanism in composite material winding process parameters and presented a quadratic regression model for the interlaminar shear strength based on RSM, yielding the optimal combination of process parameters [11]. In [12], a hybrid neural network is used to determine the optimal curing time, which can ensure complete curing of composite products.
One can see from the literature that prior research mainly focused on singleobjective optimization, but the filament winding products have multiple objectives to be evaluated. GRA is a method of multivariate statistical analysis. In general, we want to understand the strength of a project affected by other factors in a grey system. In [13–16], GRA is introduced to solve complex relations between multiple factors and variables. GRA has been successfully applied in many engineering fields, such as welding [17, 18], highspeed machining [19–22], mechanical design of positioning platforms [23, 24], and wire electrical discharge machining [25–30].
The primary work in this paper includes calculating grey correlation coefficients (GCCs) between residual stress and porosity based on experimental data. GRG can be subsequently obtained using a weighting method. A secondorder prediction model for GRG is established based on experimental data with the use of RSM. The influence of process parameters on GRG is analyzed, and the optimum combination of process parameters is obtained and verified through experiments. The results in this paper show that a particular multiobjective problem can be transformed into a singleobjective problem using GRA. The optimum combination of process parameters in the composite prepreg tape winding process can be subsequently determined, and the residual stress and void content of composite products can be controlled.
2. Experiment Procedure and Results
2.1. Composite Prepreg Tape Winding Process
In the process of composite tape winding, tension is a key process parameter. Tension is applied with a magnetic powder brake during the winding process. Tension can straighten the prepreg winding so that the fiber can bear the load evenly. The applied tension can remove air bubbles, make the winding products more compact, and facilitate resin penetration. In the winding process, the core mold rotates at a constant speed, and the resin is heated to the melting state by the hot pressure roller and the hot blower. As shown in Figure 1, heat comes from the internal heating wire in the hot pressure roller, which helps reduce the resin speed and increase the degree of contact between the layers. In the melting zone, the hot pressure roller exerts positive force on the tape layer, causing the prepreg tape and the tape layer to come into close contact. On the contrary, it helps reduce void content by reducing bubbles between interlayer contacts.
The winding of the prepreg tape is essentially a process of continuous fusion between the prepreg tape and the base layer. When a certain winding pressure and temperature are applied to the winding layer and prepreg, the surface geometry will be deformed, as shown in Figure 2. The selfbonding process begins when the winding layer is in close contact with the prepreg surface. After a period of time, the polymer chain penetrates completely and entangles with the adjacent interface so that the matrix on the interface forms the bulk polymer again, and the two surfaces are fully integrated.
2.2. Experimental Procedures
A KUKA robot (XGD1200) (KUKA, Augsburg, Germany) is the primary piece of equipment used in our experiments, as shown in Figure 3. In order to ensure the control accuracy of the winding process, a highprecision deviation correction control system and layered superposition winding are used in the experiment. Circumferential winding experiment is carried out with the orthogonal prepreg tape. T300/epoxy orthogonal prepreg tape is purchased from Daobo Composites Co., Ltd., Xi’an, China. The winding mandrel is a 45 steel cylinder which is 150 mm in external diameter and 1200 mm in length. The parameters of the prepreg tape are fiber volume fraction, tape width, and tape thickness, which are 56 ± 2%, 80 mm, and 0.25 mm, respectively. In this experiment, the ambient temperature is 20 ± 2°C, and the relative humidity is 25 ± 2%. The curing process has a great influence on the properties of the products. During the curing process, the heating rate is kept at 2.5°C/min. When the curing temperature reaches 150°C, it is needed to keep heating for 150 minutes, and the curing pressure is 0.15 MPa.
(a)
(b)
2.3. Sample Preparation and Measurement Method
2.3.1. Residual Stress
In the process of composite prepreg winding, due to the deformation of the product, the residual stress is inevitable. Residual stress is a key index to evaluate the properties of composite products, which is selected as one of the optimization objectives. When examining residual stress in composite annular parts, a slot is cut along the radial direction, and the slot position will change due to the residual stress moment. Figure 4 shows the change in slot displacement after closure of the compound ring, which can be measured with an electron microscope. The circumferential residual stress in the composite ring can be calculated with the following equations [31, 32]:where is the current position, is the total displacement of the slot, is the bending moment per unit width, is the circumferential elastic modulus, and and are the inner and outer radii, respectively.
The magnitude of the residual stress is the average value of the composite outer and inner rings, which can be defined as follows:
2.3.2. Void Content
Voids in composite tape winding products are defects that principally exist between tape layers due to residual air bubbles, resin flow, and sufficient compaction during resin flow. Density measurements, microscopy [33–39], ultrasonic attenuation [40], and Xray computed tomography [41] can be used to measure void content. The electronic micrograph method has the highest porosity detection accuracy, which is specified by GB/T33652008 [42]. The specimen is sampled and observed at the marked position, as shown in Figure 5. The samples are cut on the composite ring product, with a length, width, and height of 20 mm, 10 mm, and 10 mm, respectively. The samples are ground and polished under flowing water, then the polished specimen is observed under a microscope, and the process of measuring void content is shown in Figure 6. The calculation formula of void content is shown in the following equation:where X is the void content, A is the crosssectional area, and is the total void area of the sample.
2.4. Experiment Results
Temperature, winding speed, roller force, and winding tension are taken as the independent experimental variables, and residual stress and porosity are the response variables and design variable values according to actual working conditions. The fourfactor and threelevel BBD experiment design method was used to reduce costs. BBD is a response surface design type, which does not include embedding factor or partial factor design. BBD usually has fewer design points, and each factor always has 3 levels. According to the actual production experience, the temperature setting range is 50–100°C. When the prepreg tape temperature is lower than 50°C, the resin matrix is difficult to reach the melting state, and when the temperature is too high, it will easily lead to early curing of the resin. The pressure setting range is 1000–2000 N; when the pressure is less than 1000 N, the contact between the laminate and prepreg tape is not enough, and when the pressure is too large, the winding products will be deformed. The setting range of tension is 100–500 N; too small tension will increase the number of air bubbles between layers, and too large tension will lead to the fracture of the prepreg tape. The speed setting range is 5–15 rpm, and too fast winding speed is not conducive to machining. The designed level of process parameters is shown in Table 1, and the experimental results are shown in Table 2.


3. Grey Relational Grade Calculation from Experimental Data
3.1. GRG Calculation Process
Step 1: experimental void content and residual stress data were collected and used to carry out a standardized treatment. Composite tape winding products with lower void content and residual stress are desirable. Therefore, the experimental data can be expressed as follows:where is the original sequence, is the comparison sequence, k = 1, 2, …, n, i = 1, 2, …, m, and n and m are the total number of response variables and experimental runs. Step 2: the grey correlation coefficient can be calculated by the following equation:where is the deviation sequence, is the reference sequence, and is the distinguishing coefficient. Step 3: calculation of the weight value for response variables: in this paper, the contributions of void content and residual stress are quantified by PCA. The calculation process is expressed as follows:(a)Establishing the original sequence of various quality characteristics:where m is the number of experiments, n is the number of response variables, and x is the grey correlation coefficient of each response variable.(b)Calculation of the correlation coefficient array:where is the covariance of and and and are the standard deviations of and .(c)Computation of eigenvalues and eigenvectors: can be obtained by the following equation:where is the identity matrix and the eigenvalues are arranged in the ascending order, i.e., , k = 1, 2, …, n.(d)Calculation of weight of the principal component:Generally, and are called the first and second principal components if , respectively. Step 4: calculation of the grey relational grade: GRG is the weighted sum of the grey relational coefficient and can be calculated by the following equation:where , and is the weight of the kth response variable and determined by PCA.
3.2. Results for GRA
Principal component analysis for weight values and results for GRA are provide in Tables 3 and 4.

 
Notes: Δ_{0i}: deviation sequence; : comparison sequence; GRC: grey relational coefficient; RS: residual stress; and VC: void content. 
4. The Grey Relational Grade Prediction Model
According to PCA for weight values as shown in Table 3 and results for GRA as shown in Table 4, a mapping relation between the process parameters and the GRG can be established. Generally, a secondorder mathematical regression model in response surface methodology is used to determine the relationship between the response variable and the input factor. The secondorder GRG model for the winding process parameters can be expressed as follows:where is the estimated GRG value, is a winding process parameter, is the experimental error, and each is a secondorder regression coefficient. The second term models a linear effect, the third term models an interaction effect, and the fourth term models secondorder effects.
GRG prediction model is based on regression analysis of experimental data using Minitab software. A comparison between the predicted and calculated GRG values is shown in Figure 7. Figure 7 shows that the predicted GRG value is very close to the calculated value, with an average deviation of 1.22%. Thus, there is no significant difference between the predicted value and the calculated value. The residual error in the prediction model is shown in Figure 8, which shows that residual errors are randomly distributed near zero without abnormal points. Thus, the prediction model is a good fit to the experimental data. Analysis of variance (ANOVA) results for the prediction model are shown in Table 5. One can see from the results in Table 5 that the coefficients of determination (RSq and RSq (adj)) are very close, indicating that the model is very reliable and accurate. The prediction model is shown in the following equation:
 
Notes: DF: degree of freedom; SS: sum of square; MS: mean square; and SD: standard deviation. 
5. Multiresponse Parameter Optimization and Experimental Verification
5.1. Analysis on Parameter Influence Laws
If the GRG is larger, the response variable will be better. Correspondingly, when the average GRG value for each process parameter is the largest, the response variable is the best. Table 6 shows that the optimal level of temperature is level 3 (100°C), the optimal level of tension is level 1 (100 N), the optimal level of force is level 2 (1500 N), and the optimal level of rotation speed is level 2 (10 rpm). The difference between minimum and maximum values shows that tension has the greatest impact on the multiobjective response followed by the influence of speed, force, and temperature. Figure 9 also shows that tension has the greatest impact on residual stress, while the impact of temperature is minimal. The aforementioned parameter combination yields products with minimum residual stress.

Figure 10 shows that temperature and force have a great impact on void content, while the impact of tension is minimal. The parameter combination yielding products with minimum void content is 50°C temperature, 100 N tension, 1000 N force, and 15 rpm rotation speed. The influence of process parameters on GRG is given by the weighted sum of residual stress and void content. Therefore, the influence of process parameters on residual stress and void content can be determined by examining changes in the GRG value, and residual stress and void content can be optimized by optimizing GRG.
5.2. Optimal Parameters
The GRG prediction model is analyzed using the response optimizer in Minitab software. Figure 11 shows that the optimal GRG is 0.8106 as calculated with the weighting method, and the optimal parameter combination is 70.20°C temperature, 100.08 N tension, 1515.15 N force, and 10.25 rpm rotation speed. Figure 12 shows that the optimal GRG value is 0.8077 when calculated with the equal weight method, and the optimal parameter combination is 78.789°C temperature, 237.37 N tension, 1555.55 N force, and 9.545 rpm rotation speed.
5.3. Experimental Verification
Once the optimum combination of process parameters is determined, a confirmation experiment is conducted to validate the optimal solution. The results of the eighth experiment are used as the comparative group. Table 7 shows the comparison of winding experimental results between the initial parameter values and the optimum process parameters. The results show that the proposed method can effectively reduce the residual stress and the void content of the composite winding product.

The winding experiment is carried out with parameter combination calculated by the weighting method and parameter combination calculated by the equal weight method. Table 8 shows that the equal weight optimization parameter combination produces lower residual stress, but the void content in the product is greater than 0.95%. In order to ensure the mechanical properties of composite products, the void content should be kept at a low value, especially for special aeronautical parts. The experimental results show that the weighted method is better than the equal weight method in the winding process.

6. Conclusion
(1)The optimization of composite tape winding process parameters is a multiparameter input and multiobjective response. A procedure integrating the Box–Behnken design, RSM, and GRA is used to predict the optimal process conditions for reducing the residual stress and void content in composite products.(2)The GRG prediction model was established using Box–Behnken design based on experimental data. ANOVA results show that the prediction model is reliable and significant. The optimal combination of process parameters was found to be 70.02°C temperature, 100.08 N tension, 1515.15 N force, and 10.25 rpm winding speed. The predicted results are in good agreement with the experimental results. Residual stress and void content can be improved by using optimized parameter combination to carry out the winding process.(3)Comparing the experimental results of weighted optimal parameter combination and equal weight optimal parameter combination, the experimental results show that GRA based on equal weight has some limitations in optimizing the parameters of the composite tape winding process, and the weighted GRA method proposed in this paper has obvious advantages.
Data Availability
The data used to support the findings of this study are available from the corresponding author upon request.
Conflicts of Interest
The authors declare that they have no conflicts of interest.
Acknowledgments
This article was supported by the National Natural Science Foundation of China (grant nos. 51475377 and 51375394).
References
 P. Nimdum, B. Patamaprohm, J. Renard, and S. Villalonga, “Experimental method and numerical simulation demonstrate nonlinear axial behaviour in composite filament wound pressure vessel due to thermal expansion effect,” International Journal of Hydrogen Energy, vol. 40, no. 38, pp. 13231–13241, 2015. View at: Publisher Site  Google Scholar
 R. Rafiee, “Experimental and theoretical investigations on the failure of filament wound GRP pipes,” Composites Part BEngineering, vol. 45, no. 1, pp. 257–267, 2013. View at: Publisher Site  Google Scholar
 M. Tannous, A. Barasinski, C. Binetruy, and B. Courtemanche, “Contribution of thermomechanical parameters and friction to the bonding of thermoplastic tapes in the tape winding process,” Journal of Materials Processing Technology, vol. 229, no. 8, pp. 587–595, 2016. View at: Publisher Site  Google Scholar
 J. Grunewald, P. Parlevliet, and V. Altstadt, “Definition of process parameters for manufacturing of thermoplastic composite sandwichespart A: modelling,” Journal of Thermoplastic Composite Materials, vol. 31, no. 6, pp. 745–766, 2016. View at: Publisher Site  Google Scholar
 F. O. Sonmez and H. T. Hahn, “Analysis of the online consolidation process in thermoplastic composite tape placement,” Journal of Thermoplastic Composite Materials, vol. 10, no. 6, pp. 545–566, 1997. View at: Publisher Site  Google Scholar
 H. Lu, M. Schlottermuller, N. Himmel, and R. Schledjewski, “Effects of tape tension on residual stress in thermoplastic composite filament winding,” Journal of Thermoplastic Composite Materials, vol. 18, no. 6, pp. 469–487, 2005. View at: Publisher Site  Google Scholar
 M. Schlottermuller, H. Lu, Y. Roth, N. Himmel, R. Schledjewski, and P. Mitschang, “Thermal residual stress simulation in thermoplastic filament winding process,” Journal of Thermoplastic Composite Materials, vol. 16, no. 6, pp. 497–519, 2003. View at: Publisher Site  Google Scholar
 E. GuzmanMaldonado, N. Hamila, N. Naouar, G. Moulin, and P. Boisse, “Simulation of thermoplastic prepreg thermoforming based on a viscohyperelastic model and a thermal homogenization,” Materials & Design, vol. 93, no. 49, pp. 431–442, 2016. View at: Publisher Site  Google Scholar
 P. Xu, J. Y. Zheng, H. G. Chen, and P. F. Liu, “Optimal design of high pressure hydrogen storage vessel using an adaptive genetic algorithm,” International Journal of Hydrogen Energy, vol. 35, no. 7, pp. 2840–2846, 2010. View at: Publisher Site  Google Scholar
 P. F. Liu and J. Y. Zheng, “Strength reliability analysis of aluminiumcarbon fiber/epoxy composite laminates,” Journal of Loss Prevention in the Process Industries, vol. 23, no. 3, pp. 421–427, 2010. View at: Publisher Site  Google Scholar
 Y. Shi, T. Yu, X. He, C. Kang, X. Zhang, and J. Zhang, “Mechanism and optimization of process parameters coupling for composite tape winding,” Acta Materiae Compositae Sinica, vol. 32, no. 3, pp. 831–839, 2015. View at: Google Scholar
 R. L. Pagano, V. M. A. Calado, M. B. D. Souza, and E. C. Biscaia, “Proposal of an optimum cure cycle for filament winding process using a hybrid neural networkfirst principles model,” Polymer Composites, vol. 35, no. 7, pp. 1377–1387, 2014. View at: Publisher Site  Google Scholar
 P. Wang, Z. Q. Zhu, and Y. H. Wang, “A novel hybrid MCDM model combining the SAW, TOPSIS and GRA methods based on experimental design,” Information Sciences, vol. 345, pp. 27–45, 2016. View at: Publisher Site  Google Scholar
 R. Verma and N. P. Singh, “GRA based network selection in heterogeneous wireless networks,” Wireless Personal Communication, vol. 72, no. 2, pp. 1437–1452, 2013. View at: Publisher Site  Google Scholar
 G. Anbuchezhiyan, T. Muthuramalingam, and B. Mohan, “Effect of process parameters on mechanical properties of hollow glass microsphere reinforced magnesium alloy syntactic foams under vacuum die casting,” Archives of Civil and Mechanical Engineering, vol. 18, no. 4, pp. 1645–1650, 2018. View at: Publisher Site  Google Scholar
 P. Nanthakumar, A. Rajadurai, and T. Muthuramalingam, “Multi response optimization on mechanical properties of silica fly ash filled polyester composites using taguchigrey relational analysis,” Silicon, vol. 10, no. 4, pp. 1723–1729, 2018. View at: Publisher Site  Google Scholar
 K. S. Prasad, S. R. Chalamalasetti, and N. R. Damera, “Application of grey relational analysis for optimizing weld bead geometry parameters of pulsed current micro plasma arc welded inconel 625 sheets,” The International Journal of Advanced Manufacturing Technology, vol. 78, no. 1–4, pp. 625–632, 2015. View at: Publisher Site  Google Scholar
 J. Kundu and H. Singh, “Friction stir welding of AA5083 aluminium alloy: multiresponse optimization using Taguchibased grey relational analysis,” Advances in Mechanical Engineering, vol. 8, no. 11, pp. 1–10, 2016. View at: Publisher Site  Google Scholar
 S. T. Kumaran, M. Uthayakumar, A. Slota, and J. Zajac, “Application of grey relational analysis in high speed machining of AA (6351)SiCB_{4C} hybrid composite,” International Journal of Materials & Product Technology, vol. 51, no. 1, pp. 17–31, 2015. View at: Publisher Site  Google Scholar
 S. Y. Du, M. Chen, L. S. Xie, Z. S. Zhu, and X. N. Wang, “Optimization of process parameters in the highspeed milling of titanium alloy TB17 for surface integrity by the taguchigrey relational analysis method,” Advances in Mechanical Engineering, vol. 8, no. 10, pp. 1–12, 2016. View at: Publisher Site  Google Scholar
 J. H. Zhou, J. X. Ren, and W. J. Tian, “GreyRBFFA method to optimize surface integrity for inclined end milling Inconel 718,” The International Journal of Advanced Manufacturing Technology, vol. 91, no. 9–12, pp. 2975–2993, 2017. View at: Publisher Site  Google Scholar
 J. H. Zhou, J. X. Ren, and C. F. Yao, “Multiobjective optimization of multiaxis ballend milling Inconel 718 via grey relational analysis coupled with RBF neural network and PSO algorithm,” Measurement, vol. 102, pp. 271–285, 2017. View at: Publisher Site  Google Scholar
 S.C. Huang and T.P. Dao, “Multiobjective optimal design of a 2DOF flexurebased mechanism using hybrid approach of greyTaguchi coupled response surface methodology and entropy measurement,” Arabian Journal for Science and Engineering, vol. 41, no. 12, pp. 5215–5231, 2016. View at: Publisher Site  Google Scholar
 S.C. Huang and T.P. Dao, “Design and computational optimization of a flexurebased XY positioning platform using FEAbased response surface methodology,” International Journal of Precision Engineering and Manufacturing, vol. 17, no. 8, pp. 1035–1048, 2016. View at: Publisher Site  Google Scholar
 R. B. Azhiri, R. Teimouri, M. G. Baboly, and Z. C. Leseman, “Application of Taguchi, ANFIS and grey relational analysis for studying, modeling and optimization of wire EDM process while using gaseous media,” The International Journal of Advanced Manufacturing Technology, vol. 71, no. 1–4, pp. 279–295, 2014. View at: Publisher Site  Google Scholar
 A. Varun and N. Venkaiah, “Simultaneous optimization of WEDM responses using grey relational analysis coupled with genetic algorithm while machining EN 353,” The International Journal of Advanced Manufacturing Technology, vol. 76, no. 1–4, pp. 675–690, 2015. View at: Publisher Site  Google Scholar
 M. Thangaraj, R. Annamalai, K. Moiduddin, M. Alkindi, S. Ramalingam, and O. Alghamdi, “Enhancing the surface quality of micro titanium alloy specimen in WEDM process by adopting TGRAbased optimization,” Materials, vol. 13, no. 6, p. 1440, 2020. View at: Publisher Site  Google Scholar
 T. Muthuramalingam, “Effect of diluted dielectric medium on spark energy in green EDM process using TGRA approach,” Journal of Cleaner Production, vol. 238, Article ID 117894, 2019. View at: Publisher Site  Google Scholar
 T. Geethapriyan, K. Kalaichelvan, T. Muthuramalingam, and A. Rajadurai, “Performance analysis of process parameters on machining αβ titanium alloy in electrochemical micromachining process,” Proceedings of the Institution of Mechanical Engineers, Part B: Journal of Engineering Manufacture, vol. 232, no. 9, pp. 1577–1589, 2018. View at: Publisher Site  Google Scholar
 A. Ramamurthy, R. Sivaramakrishnan, and T. Muthuramalingam, “Taguchigrey computation methodology for optimum multiple performance measures on machining titanium alloy in WEDM process,” Indian Journal of Engineering and Materials Sciences, vol. 22, no. 2, pp. 181–186, 2015. View at: Google Scholar
 J. W. Kim and D. G. Lee, “Measurement of Residual Stresses in thick composite cylinders by the radialcutcylinderbending method,” Composite Structures, vol. 77, no. 4, pp. 444–456, 2007. View at: Publisher Site  Google Scholar
 J. W. Kim, J. H. Lee, H. G. Kim, H. S. Kim, and D. G. Lee, “Reduction of residual stresses in thickwalled composite cylinders by smart cure cycle with cooling and reheating,” Composite Structures, vol. 75, no. 1–4, pp. 261–266, 2006. View at: Publisher Site  Google Scholar
 S. Paciornik and J. D’Almeida, “Digital microscopy and image analysis applied to composite materials Characterization,” MateriaRio De Janeiro, vol. 15, no. 2, pp. 172–181, 2010. View at: Publisher Site  Google Scholar
 B. N. Fedulov, F. K. Antonov, A. A. Safonov, A. E. Ushakov, and S. V. Lomov, “Influence of fibre misalignment and voids on composite laminate strength,” Journal of Composite Materials, vol. 49, no. 23, pp. 2887–2896, 2015. View at: Publisher Site  Google Scholar
 K. Croft, L. Lessard, D. Pasini, M. Hojjati, J. Chen, and A. Yousefpour, “Experimental study of the effect of automated fiber placement induced defects on performance of composite laminates,” Composites Part AApplied Science and Manufacturing, vol. 42, no. 5, pp. 484–491, 2011. View at: Publisher Site  Google Scholar
 T. Okuya, M. Nakada, and Y. Miyano, “Reliable test method for tensile strength in longitudinal direction of unidirectional carbon fiberreinforced plastics,” Journal of Reinforced Plastics and Composites, vol. 32, no. 21, pp. 1579–1585, 2013. View at: Publisher Site  Google Scholar
 B. Deng and Y. Y. Shi, “Modeling and simulation of voids in composite tape winding process based on domain superposition technique,” Applied Composite Materials, vol. 25, no. 2, pp. 1219–1236, 2018. View at: Publisher Site  Google Scholar
 Standardization Administration of the People’s Republic of China, Test Method for Mechanical Properties of Ring of FilamentWinding Reinforced Plastics, Standardization Administration of the People’s Republic of China, Beijing, China, 2008.
 S. Paciornik and J. R. M. D’Almeida, “Measurement of void content and distribution in composite materials through digital microscopy,” Journal of Composite Materials, vol. 43, no. 2, pp. 101–112, 2009. View at: Publisher Site  Google Scholar
 H. Y. Zhu, B. C. Wu, D. H. Li, D. G. Zhang, and Y. Y. Chen, “Influence of voids on the tensile performance of carbon/epoxy fabric laminates,” Journal of Materials Science & Technology, vol. 27, no. 1, pp. 69–73, 2011. View at: Publisher Site  Google Scholar
 Y. Nikishkov, L. Airoldi, and A. Makeev, “Measurement of voids in composites by Xray computed tomography,” Composites Science and Technology, vol. 89, pp. 89–97, 2013. View at: Publisher Site  Google Scholar
 Carbon fiber reinforced plastics determination void content and fiber volume national standards of the people’s republic of China.
Copyright
Copyright © 2020 Qi Hong and Yaoyao Shi. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.